INVESTIGATION OF STORAGE CONDITIONS ON BEECH WOOD
LOGS AND CHIPS AND ITS INFLUENCE ON THE PRODUCTION OF
DISSOLVING SULFITE PULP
Andrea Promberger1, Hedda K. Weber1, Andreas Stockinger1, and Herbert Sixta2
1 Competence Center Wood, Area 6, 4860 Lenzing, Austria, Werkstrasse 1 2 Lenzing AG, BU Pulp ZF, 4860 Lenzing, Austria, Werkstrasse 1
The storage of wood is of great importance in the pulping industry for the production of dissolving pulp. Extended storage is manifested in the deterioration and discoloration of the wood, which is mostly combined with some wood loss. The resulting costs are essential factors in the pulping process. Beech wood logs have been stored for one year under dry conditions, submerged in water and irrigated, respectively. Afterwards, dissolving pulp was produced according to the acidic Mg-bisulfite pulping process. This was the basis for the evaluation of the wood quality after storage. The results were correlated with pulp from freshly cut beech wood.
Additionally, the chip storage in silos was closely investigated because of the newly equipped wood yard in Lenzing. In particular, the storage time and the
CO2-development, which is a side effect of the chip storage, were explored. Laboratory experiments were performed and compared to the chip samples from the production line as well as fresh beech wood. Furthermore, a plant trial was performed to gain better information about the wood chip storage and the quality changes during the storage period in the day-to-day production.
The water-stored wood logs showed a very good pulping performance being comparable to that of fresh beech wood. Dry stored wood, however, showed a very poor delignification and a decrease in brightness. This is attributed to highly condensed structures, which were determined with UV-microspectro-photometry.
Keywords: beech wood, storage, irrigation,
chip silo, sulfite dissolving pulp
The quality of wood is a very important aspect in the production of dissolving pulp. In the case of Lenzing, where the studies took place, primarily beech wood is used for the production of pulp by the acidic Mg-sulfite process.
The beech logs are mainly harvested in the non-growing season. This results in an extended storage period of several months before the wood is introduced into the process. The different storage methods severely influence the wood quality and the best conditions have to be found in order to guarantee a minimal quality loss. As shown
before, this seasonal variation of the wood supply significantly effects the delignification and the optical properties of both the pulp and the viscose fibers . Therefore, reinforced bleaching conditions have to be applied to compensate lower brightness, which in turn results in higher bleaching costs.
The unprotected storage of hardwood logs is accompanied by a fast decay, which affects the yield and the properties of the sulfite pulp . The effect strongly depends on the type and degree of the decay as well as on the conversion process and the
resulting final product. The demand for brighter paper from mechanical pulps and the environmental awareness are affecting the bleaching conditions and make it more important to fully utilize the potential of the raw material wood . The importance of fresh wood has also grown for the pulping processes in general . For example, the use of rotten wood increases the amount of chemicals required in Kraft pulping . Mainly fungi are responsible for the decrease in wood quality during storage. Generally, brown rot fungi depolymerize cellulose, which results in decreased fiber strength, while white rot fungi degrade lignin with fewer effects on the strength. Both types of rot degrade hemicellulose and decrease pulp yield [6, 7].
Beech wood (Fagus sylvatica L.) is
reported to be primarily attacked by white-rot fungi, such as Trametes versicolor, Pleurotus ostreatus, Lentinus edodes, only
to name a few . Recently,
Chondrostereum purpureum and Schizophyllum commune, were identified as
the two main fungal species growing on the surface of the beech logs in Lenzing [9, 10].
In addition to the long term storage of wood logs the chip storage is of great importance serving as the short term buffer in the production line. It was found that the storage time of beech wood chips significantly influences the optical properties of the pulp. The chip storage of beech wood for only four weeks resulted in a doubling of the kappa number of the unbleached pulp in the course of viscose pulp production by the sulfite process . After the introduction of a silo storage system for wood chips at the wood yard in Lenzing the maximum storage time without any quality loss had to be determined. Therefore, several process parameters like temperature, humidity, time etc. were examined.
Furthermore a microbiological characterization identified Phanerochaete chrysosporium, a white rot fungus to be
present in the chip silo .
Raw material: Freshly cut beech wood (Fagus sylvatica) was used for all log and
chip storage experiments. The long term storage was performed for one year as following:
The logs were divided into three piles. One pile was submerged in the Ager river (WET), one was continuously irrigated with water (IRR) and the third one was stored without further treatment (DRY) on fortified ground.
The fresh beech wood (FRESH) was used as a reference. All wood samples were stored at -18°C immediately after chipping. The chip storage experiments were performed with the fresh beech wood in plastic buckets with a lid in a climate chamber for 2 to 20 days. Each bucket was used for one cooking experiment. The climate chamber parameters were adjusted to 85% humidity and 40°C in order to mimic the production setup. Additionally, the chips from the production silo stored for 2 days as well as for several months were used for comparison. Furthermore, mill trials were performed storing the chips for 3 days and 6 days, respectively.
The acidic Mg-bisulfite pulping experiments were carried out in a 10L-digester according to reference .
The wood and pulp samples were analyzed by standard methods. An aliquot of the sample was taken to measure the dry content according to ISO 638-1978. The extractives content of the samples were determined with the following solvents: dichloromethane, acetone, and ethanol analog to the methods DIN 54354, ISO 624 with Soxhlet extraction and gravimetric determination of the dissolved residue. The hot water extraction was performed according to Tappi T207 om –93 and the Klason lignin isolation according to Tappi T 222 os-74 in addition to the acid soluble lignin, which is determined by the UV- VIS spectrometry .
The ash content was analyzed at 850°C combustion temperature. The cation
determination including Fe, Ca, Mn, Mg, Si, Ni, Cu was performed by ICP after microwave digestion.
The alkali resistances were analyzed according to ISO 699 / ZM IV/39/67, the carbohydrate composition by total hydrolysis and HPLC separation with AX/EC-PAD detection, the copper number according to ZM IV/8/70 and the carboxylic groups according to Das Papier
1965, 19 (1). The
UV-microspectrophotometry was performed by Koch, BFH Hamburg .
The prepared wood meal (0.5g) (FRESH, WET, IRR, DRY) was stored in sealed headspace vials at 20°, 30°, and 40°C respectively for 0 to 5 days for the CO2
-measurements. The gas phase was analyzed with a headspace (HP-7694) coupled with a GC-MS (Thermoquest-Finnigan GC-Q) and equipped with a J&W GS-GASPRO
column (30m x 0.32mm PLOT technology).
Results and Discussion
The analyses of the main wood components in the beech wood logs stored for one year (WET, IRR, DRY) are given in table 1 and are compared to the reference (FRESH). Whereas the changes in the extractives content are significant, the other parameters of the wood samples lay within the natural variation.
Parameters FRESH WET IRR DRY
DCM % 0.20 0.19 0.16 0.14 Ethanol % 1.7 0.6 0.6 0.5 Acetone % 1.0 0.4 0.4 0.3 Hot water % 2.7 1.8 1.9 1.9 Glucan % 41.6 41.9 41.7 41.0 Xylan % 17.9 17.8 18.0 19.0 Mannan % 1.3 0.5 0.5 1.1 Arabinan % 0.5 0.5 0.4 0.3 Galactan % 1.2 0.6 0.5 0.4 Klason % 21.1 21.4 20.0 20.7 Acid soluble % 3.1 3.3 4.1 3.3 Ash content % 0.34 0.38 0.41 0.32
Table 1. Wood analysis of the main components in
fresh and stored wood logs.
The results of the continuous sampling of the stored logs over the storage period
reveal a significant course in the extractives content starting with an increasing release followed by a fast deterioration of the storage substances, particularly in dry stored beech wood as given in figure 1.
Figure 1. Development of extractives in dry stored
beech wood logs over the storage period of time (days)
The samples WET and IRR, however, show only a continuous decrease in the hydrophilic extractives (not shown). These were most likely washed out, whereas the hydrophobic extractives remain constant and were comparable to the values of the dry stored sample.
A variation in the extractives was also observed for the wood chips. The change was caused by the faster deterioration of the storage substances, which were easier accessible because of the larger surface. Also a rather quick change in the wood color was determined, which could be correlated with the quality of the cooking performance: The delignification selectivity decreased with the increase of the discoloration of the wood chips, which was caused by oxidative reactions of the extractives . These results were verified with the chip storage experiments and the pulp mill trials, which are discussed below. The main interest of the investigation was the performance of the stored wood in the pulping process. Therefore, all stored samples were digested by the acidic Mg-bisulfite process and the produced pulps were analyzed. 0 0,5 1 1,5 2 2,5 3 3,5 0 50 100 150 200 days 250 [%] DCM Aceton Ethanol
Especially the log storage yielded interesting results. Again the fresh beech wood was used as the reference.
Surprisingly, the delignification selectivity of the two wet stored wood samples was excellent and well comparable to the fresh beech wood as illustrated in table 2.
Sample Visc. Bright. Kappa V/K value
ml/g % ISO # ml/g
FRESH 700 65 4.4 159
WET 700 67 4.4 160 IRR 700 63 5.2 135 DRY 700 50 7.7 91
Table 2. Viscosity/Kappa ratio of differently stored
beech wood samples at the target CED viscosity of 700ml/g
Even the irrigated wood showed a very good delignification performance. In contrast, the pulp product from the dry stored wood had the lowest brightness values and the highest kappa-numbers, resulting in the worst delignification performance.
The results of the chip storage experiments and the chips of the silo were compared with respect to their pulping performance. Again the fresh beech wood was used as the reference. The climate chamber (cc) samples (2d cc and 20d cc) and the silo samples were cooked at two different H-factors.
Despite the expectations of a gradually decreasing performance of the stored beech wood chips, all but one sample showed no negative storage effect (figure 2).
Figure 2. Delignification as correlation of viscosity
to brightness of differently stored beech wood chips from the climate chamber and the silo
The delignification of the silo samples had as expected a slight and a high decrease for the 2d and 90d stored sample, respectively. The sample from the climate chamber (20d cc), which did not follow this trend, was discolored and heavily contaminated with bacteria on the chip surface. It gave a bad result concerning the brightness and delignification performance. Although the growth of micro-organisms was limited to the chip surface, we assume that the bad pulping performance was caused by this infestation. For example the fungus C. purpureum along with other surface
growing micro-organisms can build up barriers for the cooking liquor with their hyphae and, therefore, inhibit the impregnation and penetration of the wood. Conclusively, this could result in a higher amount of residual lignin and chromophoric structures.
We assume that during the experiment the lids of the buckets were airtight excluding the 20d cc sample. This resulted in an oxygen limitation because of the respiratory activity of micro-organisms present. The atmosphere in the buckets did not suffice for a continuous growth of the various micro-organisms before long. All analysis buckets as well as the contaminated sample were reopened during that storage time and changed their color quickly, whereas the unopened samples kept their original color.
A pulp mill trial was performed with an extended storage of the wood chips in the silo for 3 and 6 days, respectively. The unbleached pulps were compared with the previously produced batch under comparable conditions. The trial data are presented in table 3.
These experiments revealed that the decrease of the brightness seemed to be high within the first 3 days but no further changes were observed for this parameter after another three days of storage. The
400 550 700 850 35 45 55 65 Brightness [%ISO] Vi scosi ty [ m l/ g]
fresh 2d cc 10d cc 20d cc 2d silo 90d silo heavily contaminated
variation of the kappa number, however, doubled between the 3rd and 6th day of storage. We presume that the high impact of these storage experiments on the pulp quality originated from a great quantity of fresh beech wood present in the silo, which has a higher concentration of extractives as described before. Additionally, the high outside temperatures during these experiments promoted the unwanted oxidation and condensation reactions in the silo .
Storage time ∆Kappa ∆ Brightness ∆ Visc.
%∆ %∆ %∆
3 days + 10,9 - 5,3 + 12,3 3 days + 17,5 - 7,3 + 4,0 6 days + 30,4 - 7,0 - 4,3 6 days + 31,6 - 5,1 + 10,6
Table 3 Percentile variation of the plant trial of 3d
and 6d chip storage in the silo in relation to the prior pulp batch
These results are comparable to the quality decrease described by Etzhold , although his investigation was made with outdoor piles over a longer period of time. Another practical aspect in the silo storage is the massive development of CO2 in the
silo, which can reach high concentrations depending on the storage time, temperature, wood quality, silo operation mode, and several other parameters.
As already mentioned the CO2
-development is dependent on the storage temperature of the wood chips (figure 3). A higher temperature resulted in an increasing CO2-concentration. We assume that the
development of CO2 has two different
sources, on one hand the increased microbial activity with the risen temperature and on the other hand the accelerated enzymatic oxidation of the extractives in the parenchyma cells at elevated temperatures as described by Koch , .
Figure 3. Cumulative CO2 concentration deriving from
freshly cut beech wood chips at different temperatures
Since the CO2 development also closely
correlated with the concentration of the extractives, it can be clearly stated that wood with high extractives content e.g. fresh beech wood produces more CO2 than
dry stored wood (figure 4).
Figure 4. Cumulative CO2 concentration in 1 year wet,
irrigated and dry stored beech wood in comparison to fresh beech wood.
The characteristic in the different storage forms was accompanied by the variation of the extractives content, which is also very important concerning the CO2
The delignification was also influenced by the storage conditions of the logs and chips. The wet and irrigated samples had a better and faster delignification performance compared to the dry stored wood. The mill
0 2 4 6 8 10 12
day 0 day 1 day 2 day 3 day 4 day 5
gCO 2 /k g wood fresh wet irr dry 0 2 4 6 8 10 12 14 16 18
day 0 day 1 day 2 day 3 day 4 day 5
g CO 2 /kg wood 20°C 30°C 40°C
trials gave a decreasing performance with increasing chip storage time.
The brightness results showed the same trend as those from the delignification. The wet and irrigated wood was comparable to the fresh samples, whereas the dry sample had a higher content of residual chromophores, highly condensed structures, which were found and further investigated by Koch with UV-micro-spectrophotometry . These substances are most likely polyphenols, which are accumulated in the cell lumina . This result is also in accordance to the blocked cell lumina reported by Hägglund and Lange .
Finally we can state that the lower degree of delignification including the  presence of highly condensed structures in the unbleached pulp negatively effected the bleaching process by demanding a higher amount of bleaching chemicals. A wet storage of the beech wood logs is definitely of advantage for the pulping process of dissolving pulp as well as a short storage time of the chips in the silo especially during the warm season.
Financial support was provided by the Austrian government, the provinces of Lower Austria, Upper Austria and Carinthia as well as by the Lenzing AG. We also express our gratitude to the Johannes Kepler University, Linz, the University of Natural Resources and Applied Life Sciences, Vienna, and the Lenzing AG for their in kind contributions. We also want to thank Dr. Gerald Koch from the BFH Hamburg, Germany for the UV-microspectrophotometric
 Sixta, H.; Promberger, A.; Koch, G.; Gradinger, C.; Messner, K.; In
International Symposium on Wood Based Materials; Wood composites
and Chemistry; Robert Stingl, ed.;
Inst. of Wood Science and Technology: Vienna, 2002; Vol. 4,
 Rydholm, S. A.; Pulping Processes,
Wiley Interscience: New York 1965.  Varhimo, A.; Tuovinen, O.; In
Mechanical Pulping, Sundholm J.,
ed.; FAPET/Tappi: Helsinki, 1999, pp. 67.
 Söderstam, G.; Öman, M.; Olofsson, J.; In STFI Renserikonferens; STFI:
STFI Stockholm, 1998.
 Henningsson, B.; Biodeterioration Materials 1972, 2, 336.
 Hunt, K.; Pulp Paper Can. 1978, 79,
 Procter, A. R.; Pulp Paper Can.
1973, 74, 62.
 Faix, O.; Bremer, J.; Schmidt, O.; Stevanovic, J.; J. Anal. Appl. Pyrolysis 1991, 21, 147.
 Promberger, A.; Sixta, H.; Gradinger, C.; Messner, K.; In 223rd ACS National Meeting; American
Chemical Society: Orlando, USA, 2002, pp. CELL 110.
 Gradinger, C., Personal Communi-cation.
 Lenz, J.; Fuhrmann, F.; Peter, W.; Geppert, K.; Lenzinger Berichte
1981, 51, 10.
 Fischer, K.; Schmidt, I.; Zellstoff und Papier 1977, 11, 344.
 Gradinger, C.; K.Messner; Promberger, A.; Sixta, H.; In 12th International Symposium on Wood and Pulping Chemistry; University of
Wisconsin, Madison, Department of Forest Ecology and Management: Madison, USA, 2003; Vol. 3, pp. 27.
 Sixta, H.; Promberger, A.; Koch, G.; Gradinger, C.; Messner, K.;
Holzforschung 2004, 58, 14.
 Sjörström, E.; Alén, R.; Analytical Methods in Wood Chemistry, Pulping and Papermaking, Springer Verlag:
 Koch, G.; Kleist, G.; Holzforschung
 Koch, G.; Bauch, J.; Puls, J.; Welling, J.; ForschungsReport 2001, 2, 30.
 Etzhold, C.; Kretzschmar, G.; Öchsner, W.; Wiessner, P.; Zellstoff und Papier 1974, 5, 131.
 Promberger, A.; 2004, Doctoral thesis, University of Technology Graz, Graz
 Koch, G.; Bauch, J.; Puls, J.; Schwab, E.; Welling, J.; Holzzentralblatt
2000, 6, 1.
 Koch, G.; Puls, J.; Bauch, J.;
Holzforschung 2003, 57, 339.
 Hägglund, E.; Lange, P. W.; Über den Sulfitaufschluß von weißfaulem Buchenholz, Report, Schwedisches Holzforschungsinstitut: Stockholm, 1950.